cleaning interfacesin layered materials heterostructures cleaning interfacesin layered materials...
Post on 15-Jun-2020
Embed Size (px)
Cleaning Interfaces in Layered Materials Heterostructures
D. G. Purdie1, N. M. Pugno2,3,4, T. Taniguchi5, K. Watanabe5, A. C. Ferrari1, A. Lombardo1∗ 1 Cambridge Graphene Centre, University of Cambridge, Cambridge CB3 0FA, UK
2 Laboratory of Graphene and Bio-inspired Nanomaterials, Department of Civil,
Environmental and Mechanical Engineering, University of Trento, Italy 3 School of Engineering and Materials Science, Queen Mary University of London, UK
4 Ket-lab, E. Amaldi Foundation, Italian Space Agency, Via del Politecnico, Rome 00133, Italy and 5 National Institute for Materials Science, 1-1 Namiki, Tsukuba 305-0044, Japan
Heterostructures formed by stacking layered materials require atomically clean interfaces. How- ever, contaminants are usually trapped between the layers, aggregating into blisters. We re- port a process to remove such blisters, resulting in clean interfaces. We fabricate blister-free re- gions of graphene encapsulated in hexagonal boron nitride of∼ 5000µm2 , limited only by the size of the exfoliated flakes. These have mobilities up to∼180000cm2V−1s−1 at room temperature, and∼ 1.8 × 106cm2V−1s−1 at 9K. We further demonstrate the effectiveness of our approach by cleaning heterostructures assembled using graphene intentionally exposed to polymers and solvents. After cleaning, these samples reach similar high mobilities. We also showcase the general applica- bility of our approach to layered materials by cleaning blisters in other heterostructures based on MoS2. This demonstrates that exposure of graphene to processing-related contaminants is compat- ible with the realization of high mobility samples, paving the way to the development of fab-based processes for the integration of layered materials in (opto)-electronic devices.
The ability to stack single layer graphene (SLG) and other layered materials (LMs) into heterostructures (LMH) has made it possible to create materials where the properties can be tailored by design[1–7]. A number of challenges remain before LMHs can be widely applied, such as the need to use LMs prepared by scalable tech- niques, like chemical vapor deposition (CVD)[8–12], and to achieve clean interfaces over the entire dimensions of the LMH. One of the most widely studied LMHs is SLG encapsulated in hexagonal boron nitride (hBN)[13–20]. hBN encapsulated SLG can achieve room temperature (RT) mobilities (µ) up to∼150000cm2V −1 s−1, over an order of magnitude higher than SLG on SiO2. Furthermore, encapsulation isolates SLG from sources of contamination, such as lithographic polymers and solvents used during device processing, or ambient air, which can otherwise degrade µ[17, 21] and in- crease doping. Thus, hBN encapsulated SLG could enable state of the art performance for a range of ap- plications in high-frequency electronics[7, 22–24], and (opto)electronics[25–27].
Encapsulated SLG and other LMHs are assembled by first producing the individual LMs on separate sub- strates, typically Si+SiO2, or polymers, such as Poly- methyl methacrylate (PMMA)[13, 28], followed by trans- fer and stacking to achieve the desired LMHs[13, 15, 28]. During stacking, contaminants such as hydrocarbons, air or water[30, 31], can become trapped between the layers, aggregating into spatially localized pockets with lateral sizes which vary from tens nm up to a few µm, known as ‘blisters’ or ‘bubbles’[14, 15, 29], which form due to the interplay of LM elastic properties
and van der Waals forces. This aggregation of contaminants into blisters
leaves the regions located between them with clean interfaces, and devices can therefore be fabricated exploiting these areas. However, the device size is constrained by the blister spacing, typically∼1-10µm. For hBN encapsulated SLG, this also limits fundamen- tal studies, since at cryogenic temperatures (T) the charge carrier mean free path in SLG, lm, can reach> 10µm[15, 16], which results in the electrical conductivity becoming limited by scattering of carriers with device edges, due to the lateral dimensions of the sample, W, being< lm. In general, the random placement of blis- ters is incompatible with scalable fabrication processes, requiring devices to be deterministically located. Thus, it is a must to develop methods to eliminate blisters. Blister-free areas> 10µm can be obtained by using
a ‘hot pick-up’ technique, where interfacial contam- inations are removed during encapsulation by bringing the layers together in a conformal manner at∼110◦C. The cleaning in this process is attributed to the higher diffusivity of the contaminants at 110◦C than at RT, allowing them to diffuse out of the sample during en- capsulation. Large blister-free regions were also reported in Ref.15, up to∼ 300µm2, although no explanation of how blisters are avoided was given. In Refs.19,15 resid- ual blisters sometimes remained within the samples due to incomplete cleaning during transfer. Furthermore, the technique of Ref. only achieves clean interfaces when the encapsulation is performed slowly, with lateral speeds< 1µm/s, limiting its applicability to scalable pro- cesses. The required time would increase as the total number of interfaces within the LMH increases. Ref.19 also produced LMHs using SLG intentionally contami- nated with PMMA residuals left from lithographic pro-
cessing, suggesting that the ‘hot pick-up’ technique could be used to exclude these polymer residuals. However, no comparison was given of µ of samples produced using clean and polymer contaminated SLG.
Here we show how to remove contaminations trapped within already assembled LMHs. This is achieved by laminating the LMH onto a SiO2 substrate at∼180◦C. At this T the blisters become physically mobile, enabling them (and the contaminants trapped inside) to be pushed to the sample edges, where they are eliminated. We achieve blister-free hBN-encapsulated SLG with lateral dimensions up to∼5000µm2, limited only by the size of the exfoliated flakes, one order of magnitude larger than Refs.15, 19. We manipulate blisters at speeds> 10µm/ s, over an order of magnitude faster than Ref.19. Our approach also allows the LMH interfaces to be cleaned simultaneously, unlike the ‘hot pick-up’, where the inter- faces need to be cleaned sequentially. Thus, our total cleaning time is independent on the number of layers. We also demonstrate blister cleaning of LMHs with MoS2, indicating the general suitability of our approach. We fabricate 4 terminal devices, exploiting the entire LMHs area, with Hall bar widths up to W = 24µm. We achieve µ up to 180000cm2 V −1s−1 at RT. µ is consistently high across all samples, with an average∼ 160000cm2 V−1s−1 across 15 Hall bars. Hall bars with µ up to∼ 150000cm2 V−1s−1 were previously reported[14, 28], but in devices with W < 3µm, limited by the blister spacing, while our technique enables µ > 100000cm2 V−1s−1 to be consis- tently achieved over the entire LMH dimensions. We re- port µ up to∼1.8×106cm2 V −1s−1 at 9K. To the best of our knowledge, this is the highest diffusively mea- sured µ in SLG, with similar values only obtained us- ing ballistic measurements where lm exceeded the sam- ple dimensions[15, 16]. We also show that our ap- proach works on SLG intentionally exposed to PMMA, acetone and isopropyl alcohol (IPA) before encapsula- tion, achieving µ up to∼150000cm2 V −1s−1 at RT af- ter cleaning, i.e., there is no µ degradation compared to non-contaminated SLG. This is significant because, to date, exposure of SLG to polymers and solvents be- fore encapsulation resulted in samples with limited µ, attributed to the contaminants trapped at the SLG-hBN interface[14, 15, 17, 28]. E.g. Ref.23 used a semi-dry transfer and achieved µ ∼ 50000cm2V−1s−1 at 1.6K, a factor∼ 35 lower than us. Ref.13 used non-encapsulated SLG on a bottom hBN, with SLG exposed to both poly- mers and solvents, followed by annealing at 300◦C to remove residuals, achieving µ 1×1012cm−2 and 7.2K, a factor∼ 40 lower than us. In Ref.28 SLG exposed to polymer and solvents before encapsulation showed µ up to∼ 150000cm2 V−1s−1 at T 100µm) SLG flakes, whereas flakes pro- duces without heating are typically < 50µm in size, in agreement with findings of Ref.40. For the exfoliation of hBN, no plasma treatment of the SiO2 surface is used, as we find this has no effect on the flakes lateral size. SLG and hBN flakes are identified prior to transfer
by a combination of optical microscopy and Raman spectroscopy[42–46]. To showcase the effectiveness of our approach, we fabricate LMHs with a range of hBN thicknesses, thBN (2-300nm), and widths, WhBN (up to∼ 200µm), observing blister manipulation and cleaning in all cases. For devices targeting µ > 100000cm2V−1s−1, we select bottom hBN flakes with thBN > 10nm, as below this value the hBN no longer screens the rough- ness of the underlying SiO2. Furthermore, thin (thBN < 10nm) hBN flakes may provide insufficient screening from charged impurities in the underlying SiO2[47, 48], and both of these factors may degrade the SLG µ. We note that, to the best of our knowledge, all µ >∼ 100000cm
2V−1s−1 samples in literature used thBN >∼ 10nm[13–15, 17, 28]. In order to pick up and transfer the flakes we use
a stamp consisting of a layer of polycarbonate (PC) mounted on a block of polydime